General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.84 g/cm³ Show Material materials with Density of 7.84 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | -100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa | |

20.0 °C | 212 GPa Show Material materials with Elastic modulus of 212 GPa | ||

100.0 °C | 207 GPa Show Material materials with Elastic modulus of 207 GPa | ||

200.0 °C | 199 GPa Show Material materials with Elastic modulus of 199 GPa | ||

300.0 °C | 192 GPa Show Material materials with Elastic modulus of 192 GPa | ||

400.0 °C | 184 GPa Show Material materials with Elastic modulus of 184 GPa | ||

500.0 °C | 175 GPa Show Material materials with Elastic modulus of 175 GPa | ||

600.0 °C | 164 GPa Show Material materials with Elastic modulus of 164 GPa | ||

Elongation | 20.0 °C | 19 % Show Material materials with Elongation of 19 % | |

Elongation, transverse | 20.0 °C | 17 % Show Material materials with Elongation, transverse of 17 % | |

Poisson's ratio | 23.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | Typical for Steel |

Tensile strength | 20.0 °C | 560 - 730 MPa Show Material materials with Tensile strength of 560 - 730 MPa | |

Tensile strength, transverse | 20.0 °C | 560 - 730 MPa Show Material materials with Tensile strength, transverse of 560 - 730 MPa | |

Yield strength | 20.0 °C | 440 - 460 MPa Show Material materials with Yield strength of 440 - 460 MPa | |

Yield strength, transverse | 20.0 °C | 440 - 460 MPa Show Material materials with Yield strength, transverse of 440 - 460 MPa |

Thermal

Property | Temperature | Value |
---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.05E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.05E-5 1/K |

20.0 °C | 1.15E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.15E-5 1/K | |

100.0 °C | 1.21E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.21E-5 1/K | |

200.0 °C | 1.27E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.27E-5 1/K | |

300.0 °C | 1.32E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.32E-5 1/K | |

400.0 °C | 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.36E-5 1/K | |

500.0 °C | 1.4E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.4E-5 1/K | |

600.0 °C | 1.44E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.44E-5 1/K | |

Unlock all property charts | ||

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) |

20.0 °C | 461 J/(kg·K) Show Material materials with Specific heat capacity of 461 J/(kg·K) | |

100.0 °C | 479 J/(kg·K) Show Material materials with Specific heat capacity of 479 J/(kg·K) | |

200.0 °C | 499 J/(kg·K) Show Material materials with Specific heat capacity of 499 J/(kg·K) | |

300.0 °C | 517 J/(kg·K) Show Material materials with Specific heat capacity of 517 J/(kg·K) | |

400.0 °C | 536 J/(kg·K) Show Material materials with Specific heat capacity of 536 J/(kg·K) | |

500.0 °C | 558 J/(kg·K) Show Material materials with Specific heat capacity of 558 J/(kg·K) | |

600.0 °C | 587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) | |

Unlock all property charts | ||

Thermal conductivity | -100.0 °C | 34.7 W/(m·K) Show Material materials with Thermal conductivity of 34.7 W/(m·K) |

20.0 °C | 39.7 W/(m·K) Show Material materials with Thermal conductivity of 39.7 W/(m·K) | |

100.0 °C | 40.9 W/(m·K) Show Material materials with Thermal conductivity of 40.9 W/(m·K) | |

200.0 °C | 41 W/(m·K) Show Material materials with Thermal conductivity of 41 W/(m·K) | |

300.0 °C | 39.9 W/(m·K) Show Material materials with Thermal conductivity of 39.9 W/(m·K) | |

400.0 °C | 38.2 W/(m·K) Show Material materials with Thermal conductivity of 38.2 W/(m·K) | |

500.0 °C | 36.1 W/(m·K) Show Material materials with Thermal conductivity of 36.1 W/(m·K) | |

600.0 °C | 33.8 W/(m·K) Show Material materials with Thermal conductivity of 33.8 W/(m·K) | |

Unlock all property charts | ||

Thermal diffusivity | -100.0 °C | 11.9 mm²/s Show Material materials with Thermal diffusivity of 11.9 mm²/s |

20.0 °C | 11 mm²/s Show Material materials with Thermal diffusivity of 11 mm²/s | |

100.0 °C | 10.5 mm²/s Show Material materials with Thermal diffusivity of 10.5 mm²/s | |

200.0 °C | 9.9 mm²/s Show Material materials with Thermal diffusivity of 9.9 mm²/s | |

300.0 °C | 9.1 mm²/s Show Material materials with Thermal diffusivity of 9.1 mm²/s | |

400.0 °C | 8.1 mm²/s Show Material materials with Thermal diffusivity of 8.1 mm²/s | |

500.0 °C | 6.9 mm²/s Show Material materials with Thermal diffusivity of 6.9 mm²/s | |

600.0 °C | 5.7 mm²/s Show Material materials with Thermal diffusivity of 5.7 mm²/s | |

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | -100.0 °C | 1.97E-7 Ω·m Show Material materials with Electrical resistivity of 1.97E-7 Ω·m |

20.0 °C | 2.62E-7 Ω·m Show Material materials with Electrical resistivity of 2.62E-7 Ω·m | |

100.0 °C | 3.13E-7 Ω·m Show Material materials with Electrical resistivity of 3.13E-7 Ω·m | |

200.0 °C | 3.85E-7 Ω·m Show Material materials with Electrical resistivity of 3.85E-7 Ω·m | |

300.0 °C | 4.7E-7 Ω·m Show Material materials with Electrical resistivity of 4.7E-7 Ω·m | |

400.0 °C | 5.69E-7 Ω·m Show Material materials with Electrical resistivity of 5.69E-7 Ω·m | |

500.0 °C | 6.85E-7 Ω·m Show Material materials with Electrical resistivity of 6.85E-7 Ω·m | |

600.0 °C | 8.2E-7 Ω·m Show Material materials with Electrical resistivity of 8.2E-7 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Aluminium | 0.02 % Show Material materials with Aluminium of 0.02 % |

Carbon | 0.2 % Show Material materials with Carbon of 0.2 % |

Chromium | 0.3 % Show Material materials with Chromium of 0.3 % |

Copper | 0.7 % Show Material materials with Copper of 0.7 % |

Manganese | 1 - 1.7 % Show Material materials with Manganese of 1 - 1.7 % |

Molybdenum | 0.1 % Show Material materials with Molybdenum of 0.1 % |

Nickel | 0.8 % Show Material materials with Nickel of 0.8 % |

Niobium | 0.05 % Show Material materials with Niobium of 0.05 % |

Nitrogen | 0.02 % Show Material materials with Nitrogen of 0.02 % |

Phosphorus | 0.03 % Show Material materials with Phosphorus of 0.03 % |

Silicon | 0.6 % Show Material materials with Silicon of 0.6 % |

Sulfur | 0.02 % Show Material materials with Sulfur of 0.02 % |

Titanium | 0.03 % Show Material materials with Titanium of 0.03 % |

Vanadium | 0.2 % Show Material materials with Vanadium of 0.2 % |